Yb<sup>3+</sup> can be much better than Dy<sup>3+</sup>: SMM properties and controllable self-assembly of novel lanthanide 3,5-dinitrobenzoate-acetylacetonate complexes.
Gavrikov, Andrey V.; Efimov, Nikolay N.; Ilyukhin, Andrey B.; Dobrokhotova, Zhanna V.; Novotortsev, Vladimir M.; Dalton transactions (Cambridge, England : 2003) 47 (2018) 6199–6209; doi:10.1039/c8dt00624e

data_7045963
_publ_section_title
;
 Yb<sup>3+</sup> can be much better than Dy<sup>3+</sup>: SMM properties
 and controllable self-assembly of novel lanthanide
 3,5-dinitrobenzoate-acetylacetonate complexes.
;
_journal_issue                   17
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              6199
_journal_page_last               6209
_journal_paper_doi               10.1039/c8dt00624e
_journal_volume                  47
_journal_year                    2018
_chemical_formula_moiety         'C38 H50 N4 O24 Tm2'
_chemical_formula_sum            'C38 H50 N4 O24 Tm2'
_chemical_formula_weight         1284.68
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   mixed
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.3
_audit_creation_date             2017-05-20T08:42:05-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_audit_update_record
;
2017-06-08 deposited with the CCDC.
2018-04-02 downloaded from the CCDC.
;
_cell_angle_alpha                69.2020(10)
_cell_angle_beta                 89.3350(10)
_cell_angle_gamma                74.1100(10)
_cell_formula_units_Z            1
_cell_length_a                   8.1770(4)
_cell_length_b                   12.1187(6)
_cell_length_c                   13.2254(6)
_cell_measurement_reflns_used    9919
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      31.4
_cell_measurement_theta_min      2.6
_cell_volume                     1173.00(10)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'SHELXS-2016 (Sheldrick, 2015)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.954
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.028
_diffrn_reflns_av_unetI/netI     0.0299
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.954
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            31341
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.954
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.163
_diffrn_reflns_theta_min         2.602
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.847
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.5948
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS 2014/5'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.819
_exptl_crystal_description       block
_exptl_crystal_F_000             636
_exptl_crystal_preparation       ', Magnetic properties'
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.08
_refine_diff_density_max         1.279
_refine_diff_density_min         -0.556
_refine_diff_density_rms         0.112
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.034
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     327
_refine_ls_number_reflns         8546
_refine_ls_number_restraints     9
_refine_ls_restrained_S_all      1.035
_refine_ls_R_factor_all          0.0302
_refine_ls_R_factor_gt           0.023
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0300P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0509
_refine_ls_wR_factor_ref         0.0539
_reflns_Friedel_coverage         0
_reflns_number_gt                7578
_reflns_number_total             8546
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8dt00624e2.cif
_cod_data_source_block           7
_cod_depositor_comments
'Adding full bibliography for 7045960--7045964.cif.'
_cod_database_code               7045963
_shelx_res_checksum              54149